#------------------------------------------------------------------------------
#$Date: 2022-09-15 12:05:42 +0300 (Thu, 15 Sep 2022) $
#$Revision: 277869 $
#$URL: file:///home/coder/svn-repositories/cod/cif/6/00/05/6000582.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_6000582
loop_
_publ_author_name
'Zavalij, L.'
'Zribi, A.'
'Chromik, R. R.'
'Pitely, S.'
'Zavalij, P. Y.'
'Cotts, E. J.'
_publ_section_title
;
 Crystal structure of Au1-xNixSn4 intermetallic alloys
;
_journal_name_full               'Journal of Alloys and Compounds'
_journal_page_first              79
_journal_page_last               85
_journal_paper_doi               10.1016/S0925-8388(01)01780-7
_journal_volume                  334
_journal_year                    2002
_chemical_formula_sum            'Au0.73 Ni0.27 Sn4'
_space_group_IT_number           68
_space_group_name_Hall           '-C 2a 2ac'
_space_group_name_H-M_alt        'C c c a :2'
_cell_angle_alpha                90.000
_cell_angle_beta                 90.000
_cell_angle_gamma                90.000
_cell_formula_units_Z            4
_cell_length_a                   6.4480
_cell_length_b                   11.6060
_cell_length_c                   6.4410
_cell_volume                     482.02
_cod_original_sg_symbol_H-M      'C c c a'
_cod_database_code               6000582
loop_
_space_group_symop_operation_xyz
x,y,z
-x+1/2,-y,z
x+1/2,-y,-z+1/2
-x,y,-z+1/2
-x,-y,-z
x-1/2,y,-z
-x-1/2,y,z-1/2
x,-y,z-1/2
x+1/2,y+1/2,z
-x+1,-y+1/2,z
x+1,-y+1/2,-z+1/2
-x+1/2,y+1/2,-z+1/2
-x+1/2,-y+1/2,-z
x,y+1/2,-z
-x,y+1/2,z-1/2
x+1/2,-y+1/2,z-1/2
loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_U_iso_or_equiv
_atom_site_disorder_assembly
_atom_site_disorder_group
Au 0 0.25 0.25 0.733(5) 0.00762(6) A 1
Ni 0 0.25 0.25 0.267(5) 0.00762(6) A 2
Sn 0.1637(3) 0.12063(1) 0.5786(3) 1 0.00762(6) . .
